#------------------------------------------------------------------------------
#$Date: 2024-10-06 10:12:13 +0300 (Sun, 06 Oct 2024) $
#$Revision: 295200 $
#$URL: file:///home/coder/svn-repositories/cod/cif/1/57/24/1572418.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_1572418
loop_
_publ_author_name
'Hassan, Nahid'
'Nagaraja, Suneetha'
'Saha, Sauvik'
'Tarafder, Kartick'
'Ballav, Nirmalya'
_publ_section_title
;
 Ultralow thermal conductivity and thermally-deactivated electrical
 transport in a 1D silver array with alternating δ-bonds.
;
_journal_issue                   38
_journal_name_full               'Chemical science'
_journal_page_first              15907
_journal_page_last               15912
_journal_paper_doi               10.1039/d4sc04165h
_journal_volume                  15
_journal_year                    2024
_chemical_formula_moiety         '2(Ag0.50 Br), C4 H12 N'
_chemical_formula_sum            'C4 H12 Ag Br2 N'
_chemical_formula_weight         341.84
_space_group_crystal_system      orthorhombic
_space_group_IT_number           71
_space_group_name_Hall           '-I 2 2'
_space_group_name_H-M_alt        'I m m m'
_atom_sites_solution_hydrogens   geom
_audit_creation_method           SHELXL-2014/7
_audit_update_record
;
2024-05-01 deposited with the CCDC.	2024-08-28 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   6.797(3)
_cell_length_b                   9.193(5)
_cell_length_c                   15.120(7)
_cell_measurement_reflns_used    3921
_cell_measurement_temperature    340(2)
_cell_measurement_theta_max      25.01
_cell_measurement_theta_min      2.59
_cell_volume                     944.8(8)
_computing_structure_refinement  'SHELXL-2014/7 (Sheldrick, 2014)'
_diffrn_ambient_temperature      340(2)
_diffrn_measured_fraction_theta_full 0.992
_diffrn_measured_fraction_theta_max 0.992
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0974
_diffrn_reflns_av_unetI/netI     0.0467
_diffrn_reflns_Laue_measured_fraction_full 0.992
_diffrn_reflns_Laue_measured_fraction_max 0.992
_diffrn_reflns_limit_h_max       8
_diffrn_reflns_limit_h_min       -7
_diffrn_reflns_limit_k_max       10
_diffrn_reflns_limit_k_min       -10
_diffrn_reflns_limit_l_max       17
_diffrn_reflns_limit_l_min       -17
_diffrn_reflns_number            5184
_diffrn_reflns_point_group_measured_fraction_full 0.992
_diffrn_reflns_point_group_measured_fraction_max 0.992
_diffrn_reflns_theta_full        25.006
_diffrn_reflns_theta_max         25.006
_diffrn_reflns_theta_min         2.593
_exptl_absorpt_coefficient_mu    10.514
_exptl_absorpt_correction_T_max  0.0971
_exptl_absorpt_correction_T_min  0.0213
_exptl_absorpt_correction_type   multi-scan
_exptl_crystal_colour            Colourless
_exptl_crystal_density_diffrn    2.403
_exptl_crystal_description       Needle
_exptl_crystal_F_000             640
_exptl_crystal_size_max          0.498
_exptl_crystal_size_mid          0.098
_exptl_crystal_size_min          0.078
_refine_diff_density_max         1.663
_refine_diff_density_min         -2.205
_refine_diff_density_rms         0.387
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.147
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     31
_refine_ls_number_reflns         500
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.147
_refine_ls_R_factor_all          0.1083
_refine_ls_R_factor_gt           0.0893
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.1697P)²+8.8057P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.2333
_refine_ls_wR_factor_ref         0.2576
_reflns_Friedel_coverage         0.000
_reflns_number_gt                402
_reflns_number_total             500
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            d4sc04165h2.cif
_cod_data_source_block           (TMA)AgBr2_340K
_cod_depositor_comments
'Adding full bibliography for 1572417--1572419.cif.'
_cod_database_code               1572418
_shelx_shelxl_version_number     2014/7
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_shelx_estimated_absorpt_t_min   0.077
_shelx_estimated_absorpt_t_max   0.494
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, -y, z'
'-x, y, -z'
'x, -y, -z'
'x+1/2, y+1/2, z+1/2'
'-x+1/2, -y+1/2, z+1/2'
'-x+1/2, y+1/2, -z+1/2'
'x+1/2, -y+1/2, -z+1/2'
'-x, -y, -z'
'x, y, -z'
'x, -y, z'
'-x, y, z'
'-x+1/2, -y+1/2, -z+1/2'
'x+1/2, y+1/2, -z+1/2'
'x+1/2, -y+1/2, z+1/2'
'-x+1/2, y+1/2, z+1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Ag1 Ag 0.7365(3) 0.5000 0.5000 0.0634(10) Uani 1 4 d S T P . .
Br1 Br 0.5000 0.2627(3) 0.5000 0.0604(10) Uani 1 4 d S T P . .
C1 C 0.5000 0.375(3) 0.746(2) 0.090(7) Uani 1 2 d S T P . .
H1A H 0.4595 0.2887 0.7767 0.135 Uiso 0.5 1 calc R U P A -1
H1B H 0.6301 0.3614 0.7228 0.135 Uiso 0.5 1 calc R U P A -1
H1C H 0.4104 0.3943 0.6984 0.135 Uiso 0.5 1 calc R U P A -1
N1 N 0.5000 0.5000 0.8083(15) 0.049(5) Uani 1 4 d S T P . .
Br2 Br 1.0000 0.5000 0.63620(16) 0.0586(11) Uani 1 4 d S T P . .
C2 C 0.673(4) 0.5000 0.862(2) 0.105(10) Uani 1 2 d S T P . .
H2A H 0.7321 0.4051 0.8611 0.158 Uiso 0.5 1 calc R U P B -1
H2B H 0.6382 0.5246 0.9219 0.158 Uiso 0.5 1 calc R U P B -1
H2C H 0.7649 0.5703 0.8398 0.158 Uiso 0.5 1 calc R U P B -1
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ag Ag -0.8971 1.1015 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Br Br -0.2901 2.4595 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
Br1 Ag1 Br1 107.23(11) . 9_666 ?
Br1 Ag1 Br2 112.91(3) . . ?
Br1 Ag1 Br2 112.91(3) 9_666 . ?
Br1 Ag1 Br2 112.91(3) . 9_766 ?
Br1 Ag1 Br2 112.91(3) 9_666 9_766 ?
Br2 Ag1 Br2 97.97(10) . 9_766 ?
Br1 Ag1 Ag1 53.62(5) . 9_666 ?
Br1 Ag1 Ag1 53.62(5) 9_666 9_666 ?
Br2 Ag1 Ag1 131.01(5) . 9_666 ?
Br2 Ag1 Ag1 131.01(5) 9_766 9_666 ?
Ag1 Br1 Ag1 72.77(11) 9_666 . ?
N1 C1 H1A 109.5 . . ?
N1 C1 H1B 109.5 . . ?
H1A C1 H1B 109.5 . . ?
N1 C1 H1C 109.5 . . ?
H1A C1 H1C 109.5 . . ?
H1B C1 H1C 109.5 . . ?
C2 N1 C2 111(3) . 2_665 ?
C2 N1 C1 111.2(10) . . ?
C2 N1 C1 111.2(10) 2_665 . ?
C2 N1 C1 111.2(10) . 2_665 ?
C2 N1 C1 111.2(10) 2_665 2_665 ?
C1 N1 C1 101(3) . 2_665 ?
Ag1 Br2 Ag1 82.03(10) . 9_766 ?
N1 C2 H2A 109.5 . . ?
N1 C2 H2B 109.5 . . ?
H2A C2 H2B 109.5 . . ?
N1 C2 H2C 109.5 . . ?
H2A C2 H2C 109.5 . . ?
H2B C2 H2C 109.5 . . ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Ag1 Br1 2.710(3) . ?
Ag1 Br1 2.710(3) 9_666 ?
Ag1 Br2 2.729(2) . ?
Ag1 Br2 2.729(2) 9_766 ?
Ag1 Ag1 3.215(4) 9_666 ?
Br1 Ag1 2.710(3) 9_666 ?
C1 N1 1.48(3) . ?
C1 H1A 0.9600 . ?
C1 H1B 0.9600 . ?
C1 H1C 0.9600 . ?
N1 C2 1.43(3) . ?
N1 C2 1.43(3) 2_665 ?
N1 C1 1.48(3) 2_665 ?
Br2 Ag1 2.729(2) 9_766 ?
C2 H2A 0.9600 . ?
C2 H2B 0.9600 . ?
C2 H2C 0.9600 . ?
